Research Article  Open Access
M. A. Matin, M. U. Tomal, A. M. Robin, N. Amin, "Numerical Analysis of Novel Back Surface Field for High Efficiency Ultrathin CdTe Solar Cells", International Journal of Photoenergy, vol. 2013, Article ID 652695, 8 pages, 2013. https://doi.org/10.1155/2013/652695
Numerical Analysis of Novel Back Surface Field for High Efficiency Ultrathin CdTe Solar Cells
Abstract
This paper numerically explores the possibility of high efficiency, ultrathin, and stable CdTe cells with different back surface field (BSF) using well accepted simulator AMPS1D (analysis of microelectronics and photonic structures). A modified structure of CdTe based PV cell SnO_{2}/Zn_{2}SnO_{4}/CdS/CdTe/BSF/BC has been proposed over reference structure SnO_{2}/Zn_{2}SnO_{4}/CdS/CdTe/Cu. Both higher bandgap materials like ZnTe and Cu_{2}Te and low bandgap materials like As_{2}Te_{3} and Sb_{2}Te_{3} have been used as BSF to reduce minority carrier recombination loss at the back contact in ultrathin CdTe cells. In this analysis the highest conversion efficiency of CdTe based PV cell without BSF has been found to be around 17% using CdTe absorber thickness of 5 μm. However, the proposed structures with different BSF have shown acceptable efficiencies with an ultrathin CdTe absorber of only 0.6 μm. The proposed structure with As_{2}Te_{3} BSF showed the highest conversion efficiency of 20.8% ( V, mA/cm^{2}, and ). Moreover, the proposed structures have shown improved stability in most extents, as it was found that the cells have relatively lower negative temperature coefficient. However, the cell with ZnTe BSF has shown better overall stability than other proposed cells with temperature coefficient (TC) of −0.3%/°C.
1. Introduction
Thinfilm polycrystalline CdTe is one of the leading materials for high efficiency, low cost, and stable PV cells. CdTe has a direct bandgap (Eg = 1.45 eV) which is very close to optimum bandgap (Eg = 1.5 eV) for solar cell as discussed by Shockley and Queisser [1]. It has a high absorption coefficient of 5 × 10^{5}/cm, which indicates that efficient collection of photons with energy greater than the bandgap (Eg) is possible within a very thin CdTe absorber layer as discussed by Hädrich et al. [2]. Already, the CdTe PV cell has gained a lot of attraction to the researchers and commercials for its low cost, higher efficiency, high stability, and large scale fabrication opportunity as discussed by Bätzner et al. [3]. Commercially available leading CdTe cell has an efficiency of 16.5% as discussed by Wu [4]. This cell uses a modified structure of CTO/ZTO/CdS/CdTe/Cu:HgTe:Cu_{X}Te having 10 μm CdTe and 0.1 μm CdS layer. Recently First Solar announced a new world record for CdTe photovoltaic (PV) cell having an efficiency of 18.7% as discussed on the website [5], which is quiet inferior compared to the theoretical maximum efficiency (29%). This inferiority is primarily caused because the open circuit voltage ( V) is well below what is expected for its bandgap (1.45 eV). Another critical issue related to the CdTe solar cell technology is the formation of an efficient, stable, low resistance, and nonrectifying ohmic contact on the pCdTe layer as discussed by Romeo et al. [6], since CdTe is a ptype semiconductor with a high bandgap (1.45 eV) and high electron affinity ( eV). Typically a stable ohmic contact to CdTe requires either a metal with a work function of more than 5.7 eV or a sufficiently narrow Schottky barrier to enable tunneling. There is no metal having such high work functions to make good ohmic contacts to pCdTe; instead they tend to form Schottky or blocking barriers as discussed by Partain [7]. Generally Cu is used as back contact, but back contacts containing Cu are not stable; it leads to efficiency degradation with time due to Cu diffusion to the front contact which causes shunting effect as discussed by Batzner et al. [8]. There are many allowed states within the forbidden gap at the back surface in CdTe solar cell, and recombination can efficiently take place through these states. When the minority carrier diffusion length is longer than the cell thickness, back surface recombination may become the primary limitation on cell performance. The use of an electron reflector is a strategy to overcome these obstacles. An electron reflector is a conduction band energy barrier at the back surface of the solar cell, which can reduce the recombination due to the electron flow to the back surface and helps formation of stable back contact. Typical techniques to create an efficient and stable back contact are as follows: (i)to moderate the width of conduction band barrier height for reflecting the electron by heavily doping an extra layer of back surface field (BSF) with appropriate material;(ii)to reduce the valence band barrier height between the CdTe absorber layer and final metal back contact for smooth transition of hole flow to the back contact.
Among these, the use of BSF layers at back surface has been found to be quiet easy and efficient. The importance of BSF layers attracted some attention in the 1980s as discussed elsewhere [9–11]. The BSF layer accommodates the photogenerated minority carriers and keeps them within the reach of the pn junction for efficient collection.
ZnTe is the most common BSF material. It is a ptype semiconductor having a direct band gap of 2.26 eV. Due to its lower work function and the ability to dope it highly ptype, formation of ohmic contacts to ZnTe is much easier. Bätzner et al. at the University of Parma (Italy) has proposed two more potential BSF materials for CdTe solar cells; these are Sb_{2}Te_{3} as discussed by Bätzner et al. [3] and As_{2}Te_{3} as discussed by Romeo et al. [12]. Sb_{2}Te_{3} ( eV) and As_{2}Te_{3} ( eV) both are ptype semiconductor with a low optical band gap. Another potential BSF material is Cu_{2}Te which has a moderate band gap of 1.18 eV as discussed by Hossain et al. [13]. Throughout this study using “AMPS1D” simulator, we aimed to achieve higher efficiency using BSF and study the overall effect of zinc telluride (ZnTe), antimony telluride (Sb_{2}Te_{3}), arsenic telluride (As_{2}Te_{3}), and copper telluride (Cu_{2}Te) on cell performance. The effect of temperature variation is also described to understand the environmental effect on the cell performance. This analysis indicates that As_{2}Te_{3}, Sb_{2}Te_{3}, and Cu_{2}Te are suitable BSF materials for higher efficiency (>19%) and ultrathin (<1 μm) CdTe cells. However, while considering the performances of the cell, the cell with ZnTe BSF has shown better stability than other cells.
2. Modeling and Simulation
The purpose of numerical modeling and simulation in photovoltaic cell analysis is to check the validity of proposed physical structures maintaining cell geometry and cell performance. The AMPS1D program has been developed to visualize the details of the physical operation of solar cells. The simulator has also been tested for thin film CIGS and CdTe solar cells as discussed by Degrave et al. [14]. It perfectly simulates the electrical characteristics of the thin film heterojunction solar cells. Recently, more than 200 groups worldwide have been using AMPS1D in order to design solar cell as discussed by Zhu et al. [15]. Onedimensional AMPS1D simulator has been used to investigate the effect of different BSF on ultrathin CdTe solar cell.
The baseline structure of CdTe cell as discussed by Gloeckler et al. [16] was initially modified by adding an extra layer of Zn_{2}SnO_{4} (200 nm) between SnO_{2} (TCO) and CdS layer. The additional layer of highresistiance Zn_{2}SnO_{4} is known as buffer layer. By incorporating a very thin resistive buffer layer, the CdS layer thickness can be further reduced down to <50 nm, which significantly improves the blue response, CdS film morphology, and conversion efficiency of the CdTe solar cell as discussed by MoralesAcevedo [17]. The structure SnO_{2}/Zn_{2}SnO_{4}/CdS/CdTe/Cu shown in Figure 1(a) has been taken as reference structure for this study with CdS thickness of 60 nm.
(a)
(b)
The reference cell has been further modified to Glass/SnO_{2}/Zn_{2}SnO_{4}/CdS/CdTe/BSF/Metal structure for higher conversion efficiency, shown in Figure 1(b). BSF layers have been added to overcome rollover effect, to improve stability at higher operating temperature, and to reduce the loss due to minority carrier recombination at the back contact in ultrathin CdTe cells. BSF materials used in this study are zinc telluride (ZnTe), antimony telluride (Sb_{2}Te_{3}), arsenic telluride (As_{2}Te_{3}), and copper telluride (Cu_{2}Te). For the low cost aspect, cheaper metal (Ni, Cu, and Mo) has been used as final back contact in the proposed structure. The doping concentration (up to 10^{14} cm^{−3}) used in the reference case has been changed to up to 10^{16} cm^{−3} as it is the present achievable value for CdTe material. To understand the stability of the cell, the operating temperature has been changed from 25°C to 100°C.
Table 1 shows the significant material parameters used in this modeling. The values of Table 1 were selected from standard literatures and from theoretical and practically variable values. The reference structure was the starting point of the analysis. In this modeling, the CdTe absorber layer thickness has been varied from 100 nm to up to 5 μm; all other layers thickness has been kept constant.

3. Results and Discussion
3.1. Reference Cell Simulation
The cell shown in Figure 1(a) also mentioned as reference cell has been analyzed initially. The reference cell has shown the highest conversion efficiency of 16.88% ( V, mA/cm^{2}, and ) where layer thickness of CdTe is 5 μm, layer thickness of CdS is 60 nm, and layer thickness of Zn_{2}SnO_{4} is 200 nm and Cu has been used as the back contact metal. CdTe doping concentration (5 × 10^{16}) and life time (1.6 ns) have been adopted which is the today’s achievable limit as discussed by Amin et al. [18].
Theoretically a 2 μm thick CdTe layer is efficient to absorb 99% of the incident photons with energy greater than Eg as discussed by Wu [4]. Although to avoid pinhole formation and uniformity limitation, in most high efficiency CdTe solar cells, the CdTe absorber layer is intentionally set at a minimum thickness of 5 μm. Further numerical analysis has been done using AMPS1D to reduce the thickness of CdTe layers aiming to reduce the materials usages and cell production cost. The CdTe absorber thickness has been varied from 100 nm to 5000 nm for both reference and modified cells to explore possibilities of ultrathin CdTe absorber layer. The simulated results are graphically shown in Figure 2.
Figure 2 shows that, for the reference cell, all the solar cell output parameters are unaffected for the CdTe thickness of greater than 2 μm and nearly affected around CdTe thickness of 1 μm. Further reduction of CdTe thickness below 1 μm shows that, with reduced thickness, and decreased slowly while FF increased below 500 nm. The decreases sharply at CdTe thickness of less than 0.5 μm due to critically short minority carrier diffusion length, but FF shows an increased value due to the bulk resistance reduction. All these effects result in reduction of cell conversion efficiency for CdTe absorber thickness below 1 μm. These results are in good agreement with related published works for CdTe cells as discussed by Amin et al. [18]. So having a thin CdTe layer for the reference cell is not possible while maintaining higher conversion efficiency. However, there are possibilities of increasing , , and FF below CdTe thickness of 1 μm while having improved efficiency. In order to attain this goal the reference structure has been modified with a layer of BSF (200 nm) just after the CdTe layer. The proposed structure has been shown in Figure 1(b).
3.2. Effect of BSF on Reference Cell Output Parameters
3.2.1. Effect of BSF on Short Circuit Current Density
Figure 3 graphically interprets the effect of different BSF layers on the proposed structure. The simulated figure shows that BSF has significant effect on proposed cell as it shows increase in short circuit current in small scale. The effect of BSF is quiet significant, while the absorber thickness is below 1 μm. Here BSF works as a minority carrier reflector and reduces the minority carrier recombination at back contact. As there are more carriers to contribute to , the use of BSF certainly improves cell short circuit current density. This is in a good agreement with previous work [18]. As shown above in Figure 3 the cell with zinc telluride (ZnTe) as BSF has shown most significance in improving for absorber thickness of up to 0.5 μm, whereas As_{2}Te_{3}, Cu_{2}Te, and Sb_{2}Te_{3} have shown steady, improved with variation of absorber thickness and are almost identical to each other. From the results it is evident that, with a BSF layer, a reasonable can be maintained while having an absorber thickness below 1 μm.
3.2.2. Effect of Back Surface Field on Open Circuit Voltage
Numerical analysis has been done with the proposed ultrathin cell structure SnO_{2}/Zn_{2}SnO_{4}/CdS/CdTe/BSF/BC aiming to explore the effect of different BSF materials on open circuit voltage . For realizing the effect of BSF on modified CdTe cell open circuit voltage for different BSF materials is represented graphically taking the base cell parameters as reference with a variable absorber layer thickness in Figure 4.
The effect of back surface material on open circuit voltage is found when CdTe layer thickness is <2 μm. Considerable impact is found by reducing CdTe absorber thickness below 1 μm. As in Figure 4 it can be seen that is improved significantly below CdTe layer thickness of 1 μm. This might be attributed to the reduction of the minority carrier recombination losses at the back contact in ultrathin CdTe cell. In improving , uses of arsenic telluride (As_{2}Te_{3}) as BSF have shown more significance than ZnTe, Sb_{2}Te_{3}, and Cu_{2}Te, while Sb_{2}Te_{3} and Cu_{2}Te have shown almost the same effect on . It is significant that a desired improvement in is possible although the absorber is reduced below 1 μm with just a 200 nm of BSF layer.
3.2.3. Effect of Back Surface Field on Field Factor, FF
The fill Factor also gets some changes due to the use of BSF materials. Fill factor increases with the reduction of absorber layer thickness as bulk resistance of materials has been reduced. As shown in Figure 5.
The cell with antimony telluride (Sb_{2}Te_{3}) as BSF has most significant effect on fill factor. Use of antimony telluride (Sb_{2}Te_{3}) as BSF increases fill factor below absorber thickness of 1 μm but shows a decreased value for greater absorber layer thickness. For As_{2}Te_{3}, Cu_{2}Te, and ZnTe fill factor slightly increases, while the absorber thickness is below 1 μm.
3.2.4. Effect of Back Surface Field on Overall Cell Efficiency
The effect of different BSF materials on overall conversion efficiency of modified CdTe cell has also been analyzed using AMPS1D simulator for the proposed ultrathin CdTe PV cell. The effect of BSF on overall cell conversion efficiency is represented graphically along the reference cell efficiency with a variable absorber layer thickness in Figure 6.
It is evident from Figure 6 that, when ZnTe is inserted as a BSF, the conversion efficiency does not improve significantly. Although the FF of the cell with ZnTe, as shown in Figure 5, was strongly affected, the improved as shown in Figure 3 a bit due to reduced minority carrier recombination loss at the back contact. It is clear from band diagram of the cells that the ZnTe has shown a barrier at the valence band of CdTe and ZnTe interface. The reduction in FF might be attributed to the barrier developed for holes in the valence band. These results are in good agreement with what was discussed by Amin et al. [18]. All in all, the decrease in FF dominates over the increase of ; as a result there is no significant improvement in the cell overall efficiency when ZnTe is used as BSF.
When Sb_{2}Te_{3}, As_{2}Te_{3}, and Cu_{2}Te were inserted as BSF, the conversion efficiency improved significantly with reduced absorber thickness. The improvement in efficiency of this cell came from the improvement of all the cell output parameters like FF, , and , as shown in the figures earlier. From Figure 6 it is also seen that back surface material affects cell conversion efficiency significantly when CdTe layer thickness is <1 μm. It is evident that the As_{2}Te_{3} BSF has shown the highest improvement on conversion efficiency as shown in previous figure. Sb_{2}Te_{3} and Cu_{2}Te have shown moderate improvement on cell conversion efficiency. The most important thing to be noted from Figure 6 is that the efficiency limitation with reduced absorber layer thickness discussed earlier has been overcome by the insertion of just 0.02 μm thin BSF layer.
3.2.5. Characteristics with Back Surface Field on Cell
() characteristic of a solar cell refers to the combined effect of series resistance and shunt resistance. For the better performance of solar cell higher shunt resistance is desirable, but higher series resistance is not acceptable as it might decrease the fill factor. The BSF material has great influence in characteristics, as shown in Figure 7. From the figure it is seen that the base cell curve starts rolling down around and shows maximum power at a lower value for between 0.7 V to 0.8V. But modified cell with BSF has shown noticeable increased value and better performance than base cell.
As can be seen in the figure, the structure with BSF shows higher than the cell without BSF, while the cell with ZnTe shows higher but poor FF. The FF is affected because of the higher series resistance added by the bulk resistance of the higher bandgap and the barrier for holes in the valence band and lower dielectric property of the ZnTe material. The cells with Sb_{2}Te_{3} and Cu_{2}Te have shown moderate effect of parasitic resistance on its output parameters. In this analysis arsenic telluride (As_{2}Te_{3}) has shown improved performances better than others and obtains curve almost identical to ideal curve with a negligible effect from parasitic resistances.
3.2.6. Effect of Back Surface Field on Cell Stability
Before finalizing any conclusion, the stability of the proposed cell at higher operating temperature has been investigated. Theoretically, it is expected that higher operating temperature affects cell parameters such as the band gaps, carrier concentrations, density of states, and electron and hole mobility. Similar results have also been found in this analysis. An investigation was conducted utilizing AMPS1D at operating temperature ranging from 25°C to 100°C for the proposed cells. The results obtained from AMPS1D simulation are shown in Figure 8.
The figure indicates that the conversion efficiency of both reference and proposed cells linearly decreased with the increase of operating temperature. The temperature coefficient (TC) of reference cell is found to be −0.4%/°C, which is in good agreement with theoretical evidences and related works as discussed elsewhere [13, 18, 19]. Moreover, Cells with Sb_{2}Te_{3} give better stability as its efficiency remains almost unchanged in the operating temperature range from 25°C to 50°C, and then it decreases with a TC of −0.4%/°C. The stability of cell with As_{2}Te_{3} showed the same stability of the cell without BSF. Thus, the As_{2}Te_{3} has no effects on the cell stability at higher operating temperature. The cell with Cu_{2}Te has shown improved stability more than the cell without BSF as the temperature coefficient (TC) is found to be around −0.35%/°C, whereas the cell with ZnTe showed better stability with TC of −0.3%/°C.
4. Comparison of Different BSF in Ultrathin CdTe Cells
By analysing all the graphs of different BSF materials from the previous sections it is evident that they all have similar effect on cell performance. But the numerical value of different performance parameter varies for different BSF material. Maximum efficiencies of different proposed structures with the optimum CdTe layer thickness are listed on Table 2.

Maximum conversion efficiency of cells with different BSF is found for CdTe thickness of just 0.6 μm. It is also found from Table 2 that in the proposed cell with ZnTe as a BSF the conversion efficiency (18.37%) drops more than the reference cell as the FF was strongly affected, but the improved a bit due to reduced minority carrier recombination loss at the back contact. The reduction in FF might be attributed to the band defect in ZnTe structure. When Sb_{2}Te_{3} was inserted as BSF layer, the FF and conversion efficiency improved better than that of ZnTe BSF. The As_{2}Te_{3} BSF produced best cell performances and highest conversion efficiency of 20.78%. The improvement in efficiency of this cell came from the improvement of all the cell output parameters like FF, , and . Use of Cu_{2}Te results in a moderate conversion efficiency of 19.54%. Figure 9 shows the band diagram for different proposed structures.
5. Conclusion
It has been seen that, without BSF, thinning is not possible while maintaining higher efficiency. Most important thing to be noted from the results is that the efficiency limitation with reduced absorber layer thickness has been overcome by the insertion of 200 nm thin BSF layer. From the analysis it is evident that 0.6 μm thick CdTe absorber layer is possible with acceptable range of efficiency for the proposed structure with BSF. A highly efficient (20.78%) ( V, mA/cm ^{2}, and FF = 0.84) ultrathin CdTe solar cell with 0.6 μm of CdTe, 100 nm SnO_{2}, 200 nm of Zn_{2}SnO_{4}, 60 nm of CdS, and 200 nm of As_{2}Te_{3} has been obtained. Sb_{2}Te_{3} and Cu_{2}Te as BSF are suitable for higher efficiency (>19%) and ultrathin CdTe cell. Cells with ZnTe have shown comparatively inferior performance with an efficiency of 18.37%. Cells with Sb_{2}Te_{3} gives improved stability as its efficiency remains almost unchanged in the operating temperature range from 25°C to 50°C, and then it decreases with a TC of −0.4%/°C. The cell with Cu_{2}Te shows moderate stability with TC of −0.35%/°C. As_{2}Te_{3} has no effect on stability as the TC is same as that of the reference cell. Although cell with ZnTe is the most stable cell, but while considering efficiency and stability, structures with SnO_{2}/Zn_{2}SnO_{4}/CdS/CdTe/As_{2}Te_{3}/Cu are proven to be comparable to other reported cells.
These results could open new window for ultrathin CdTe cell development and possibly lead to some improvement like: thinner absorber layer with significant performance, reduced material consumption for cell fabrication, and reduced cell fabrication cost; low cost materials (Cu, Al, and Ni) could be used as final back contact without interrupting cell performance and stability. In order to realize the possibilities, this proposed cell can further be investigated using standard fabrication technique for practical implementation.
References
 W. Shockley and H. J. Queisser, “Detailed balance limit of efficiency of pn junction solar cells,” Journal of Applied Physics, vol. 32, no. 3, pp. 510–519, 1961. View at: Publisher Site  Google Scholar
 M. Hädrich, C. Kraft, C. Löffler, H. Metzner, U. Reislöhner, and W. Witthuhn, “Pathways to thin absorbers in CdTe solar cells,” Thin Solid Films, vol. 517, no. 7, pp. 2282–2285, 2009. View at: Publisher Site  Google Scholar
 D. L. Bätzner, A. Romeo, H. Zogg, R. Wendt, and A. N. Tiwari, “Development of efficient and stable back contacts on CdTe/CdS solar cells,” Thin Solid Films, vol. 387, no. 12, pp. 151–154, 2001. View at: Publisher Site  Google Scholar
 X. Wu, “Highefficiency polycrystalline CdTe thinfilm solar cells,” Solar Energy, vol. 77, no. 6, pp. 803–814, 2004. View at: Publisher Site  Google Scholar
 2013, http://investor.firstsolar.com/releasedetail.cfm?ReleaseID=743398.
 N. Romeo, A. Bosio, R. Tedeschi, A. Romeo, and V. Canevari, “Highly efficient and stable CdTe/CdS thin film solar cell,” Solar Energy Materials and Solar Cells, vol. 58, no. 2, pp. 209–218, 1999. View at: Publisher Site  Google Scholar
 L. D. Partain, Solar Cells and Their Applications, John Wiley & Sons, New York, NY, USA, 1995.
 D. L. Bätzner, R. Wendt, A. Romeo, H. Zogg, and A. N. Tiwari, “Effect of back contact metallization on the stability of CdTe/CdS solar cells,” in Proceedings of the 16th European Photovoltaic Solar Energy Conference and Exhibition, p. 353, Glasgow, UK, May 2000. View at: Google Scholar
 R. P. Gale, J. C. C. Fan, G. W. Turner, and R. L. Chapman, “A new highefficiency GaAs solar cell structure using a heterostructure backsurface field,” in Proceedings of the 17th IEEE Photovoltaic Specialists Conference, pp. 1422–1425, New York, NY, USA, 1984. View at: Google Scholar
 P. D. Demoulin, M. S. Lundstrom, and R. J. Schwartz, “Backsurface field design for n(+)p GaAs cells,” Solar Cells, vol. 20, no. 3, pp. 229–236, 1987. View at: Google Scholar
 P. D. DeMoulin and M. S. Lundstrom, “Projections of GaAs solarcell performance limits based on twodimensional numerical simulation,” IEEE Transactions on Electron Devices, vol. 36, no. 5, pp. 897–905, 1989. View at: Publisher Site  Google Scholar
 N. Romeo, A. Bosio, S. Mazzamuto, A. Romeo, and L. VaillantRoca, “High efficiency CdTe/CdS thin film solar cells with a novel back contact,” in Proceedings of the 22nd European Photovoltaic Solar Energy Conference, pp. 1919–1927, Milan, Italy, 2007. View at: Google Scholar
 M. D. S. Hossain, N. Amin, M. A. Matin, M. M. Mannir Aliyu, T. Razykov, and K. Sopian, “A numerical study on the prospects of high efficiency ultra thin ZnxCd1xS/CdTe solar cell,” Chalcogenide Letters, vol. 8, no. 4, pp. 263–272, 2011. View at: Google Scholar
 S. Degrave, M. Burgelman, and P. Nollet, “Modelling of polycrystalline thin film solar cells: new features in scaps version 2.3,” in Proceddings of the 3rd World Conference on Photovoltaic Energy Conversion, pp. 487–490, May 2003. View at: Google Scholar
 H. Zhu, A. K. Kalkan, J. Hou, and S. J. Fonash, “Applications of AMPS1D for solar cell simulation,” AIP Conference Proceedings, vol. 462, pp. 309–314, 1999. View at: Publisher Site  Google Scholar
 M. Gloeckler, A. L. Fahrenbruch, and J. R. Sites, “Numerical modeling of CIGS and CdTe solar cells: setting the baseline,” in Proceddings of the 3rd World Conference on Photovoltaic Energy Conversion, pp. 491–494, May 2003. View at: Google Scholar
 A. MoralesAcevedo, “Thin film CdS/CdTe solar cells: research perspectives,” Solar Energy, vol. 80, no. 6, pp. 675–681, 2006. View at: Publisher Site  Google Scholar
 N. Amin, M. A. Matin, M. M. Aliyu, M. A. Alghoul, M. R. Karim, and K. Sopian, “Prospects of back surface field effect in ultrathin highefficiency CdS/CdTe solar cells from numerical modeling,” International Journal of Photoenergy, vol. 2010, Article ID 578580, 8 pages, 2010. View at: Publisher Site  Google Scholar
 M. A. Matin, M. M. Aliyu, A. H. Quadery, and N. Amin, “Prospects of novel front and back contacts for high efficiency cadmium telluride thin film solar cells from numerical analysis,” Solar Energy Materials and Solar Cells, vol. 94, no. 9, pp. 1496–1500, 2010. View at: Publisher Site  Google Scholar
 M. A. M. Bhuiyan, N. Amin, and K. Sopian, “Effects of absorber and window layer thickness on CdS/CdTe thin film solar cells from numerical analysis by SCAPS 1D,” in Proceedings of the IEEE Regional Student Conference on Research and Development (SCOReD '08), p. 210, UTM, Johor, Malaysia, 2008. View at: Google Scholar
 M. A. Matin, N. Amin, A. Zaharim, and K. Sopian, “Ultra thin high efficiency CdS/CdTe thin film solar cells from numerical analysis,” in Proceedings of the 8th WSEAS International Conference on Nonlinear Analysis, Nonlinear Systems and Chaos (NOLASC '09), pp. 338–344, La Laguna, Spain, July 2009. View at: Google Scholar
 M. A. Matin, N. Amin, A. Islam, K. Sopian, and K. K. Chong, “Effect of structural variation in cadmium telluride thin film solar cells from numerical analysis,” in Proceedings of the 24th European Photovoltaic Solar Energy Conference, pp. 3072–3076, Hamburg, Germany, 2009. View at: Google Scholar
 P. Mahawela, G. Sivaraman, S. Jeedigunta et al., “IIVI compounds as the top absorbers in tandem solar cell structures,” Materials Science and Engineering B, vol. 116, no. 3, pp. 283–291, 2005. View at: Publisher Site  Google Scholar
 M. A. Matin, N. Amin, A. Zaharim, and K. Sopian, “A study towards the possibility of ultra thin Cds/CdTe high efficiency solar cells from numerical analysis,” WSEAS Transactions on Environment and Development, vol. 6, no. 8, pp. 571–580, 2010. View at: Google Scholar
Copyright
Copyright © 2013 M. A. Matin et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.